Condensed Matter Physics, 2004, Vol. 7, No. 2(38), pp. 265–274

Electronic transport properties of compounds with temperature unstable intermediate valence of Ce M.D.Koterlyn ∗ 1,2 , R.I.Yasnitskii 1 , B.S.Morokhivskii 1 1

Ivan Franko National University of Lviv, Dragomanova Str. 50, 79005 Lviv, Ukraine

2

Academy of Bydgoszcz, Sq. Weyssenhoffa 11, 85-072 Bydgoszcz, Poland

Received March 12, 2004 Results of a thermoelectric power component (Sf ) and electrical resistivity (ρf ) measurements connected with the temperature unstable intermediate valence of Ce are presented for CeNi, CeNi2 and CeNi2 Si2 compounds in the temperature range 4–800 K. It is shown that dependences Sf (T ) and ρf (T ) are well described in a wide temperature range within the framework of a simple model of a narrow peak in the density of states gf (E) of Lorentzian shape near the Fermi level. The width of the peak depends on temperature and defines the characteristic single-ion Kondo temperature TK . Key words: rare earth compounds, valence fluctuation, electrical resistivity, thermoelectric power PACS: 72.20.Lp, 72.10.Fk, 75.30.Mb

1. Introduction Metallic systems containing rare-earth elements with unstable 4f -electronic states have been very attractive for the last decades. A speciﬁc feature of this class of compounds turns out to be the anomalously high values of certain physical characteristics, e.g., the coeﬃcient γ of the electronic-speciﬁc heat, magnetic susceptibility χ, thermoelectric power S, that can exceed the values typical of simple metals by 10 − 103 times [1,2]. In the band energy representation, a formation of the resonance peaks of the density of f -states, gf (E), near the Fermi level EF with a width of the order of the characteristic single-ion Kondo temperature TK (the so-called Abrikosov-Suhl resonance [2]) corresponds to this phenomenon. Despite the presence of a large number of experimental and theoretical works devoted to the many-body ∗

E-mail: [email protected]

c M.D.Koterlyn E-mail: [email protected] , R.I.Yasnitskii, B.S.Morokhivskii

265

M.D.Koterlyn, R.I.Yasnitskii, B.S.Morokhivskii

eﬀect studies when the conduction electrons interact with the 4f electrons in the compounds of this class, the nature of the resonant structure of the gf (E) remains the main issue to be discussed in future. Of special interest herein there are the intermetallic compounds showing the temperature unstable intermediate valence (IV) of Ce. These are most suitable for a model description in a study of the formation mechanism of the gf (E) structure. Transport properties of metallic compounds containing Ce with unstable f electrons turn out to be most sensitive to the peculiarities of the near Fermi state spectrum and can be used as a “ﬁne instrument” while studying the nature of the ground state. It is known that transport characteristics of such systems can be described in the relaxation time approximation with allowing for the exchange scattering of conduction electrons on local f -states [3–5]. However, with a detailed consideration of a number of important factors, such as the f -state orbital degeneracy, crystal ﬁeld-split f -states, the f -state hybridization with the band electrons, many-body eﬀects connected with f -electron correlation eﬀects, one cannot succeed in obtaining a general solution of the transport coeﬃcient behavior problem in a wide temperature range [6,7]. Moreover, one cannot succeed in coordinating the results of description of the transport coeﬃcients with the data of measurements of other physical properties. All this contributed to the development of a number of phenomenological approaches to the description of transport properties of such systems [8–10]. However, detailed comparisons of calculation values of transport properties within the limits of approximations [8–10] with experimental ones in a wide temperature range have not been carried out yet. This caused an insuﬃcient study of the possible usage of such experimental data for the determined resonance structure gf (E) parameters in a wide temperature range. The given paper shows temperature dependences of the contribution of Ce f states to the total thermoelectric power (Sf ) and to the electrical resistivity (ρf ) for compounds CeNi, CeNi2 and CeNi2 Si2 with diﬀerent temperature stability IV of Ce. Based on the phenomenological approach oﬀered by us earlier [10–12] there was carried out the analysis of Sf (T ), ρf (T ) dependences as well as of the transformation of the resonance structure gf (E) near the Fermi level at temperature changes within the largest limits (4–800 K).

2. Experimental data Preparation of polycrystalline samples and methods of the performed measurements were described in pervious papers [13,14]. Transport properties of the compounds CeNi, CeNi2 , CeNi2 Si2 and the corresponding analogs with La were partially analysed by us earlier [13–16]. The thermoelectric power of compounds with Ce is positive and reveals a typical maximum. The electrical resistivity manifests essential discrepancies from the Bloch-Gr¨ uneisen law characteristic of the systems with IV of Ce. For compounds with La, the thermoelectric power and electrical resistivity behavior is similar to that observed in non-magnetic transition metals. Assuming that the resistivity of the lanthanum-based counterpart can be taken 266

Electronic transport properties of compounds . . .

as a good approximation of the phonon contribution to the total measured resistivity of CeNi, CeNi2 and CeNi2 Si2 we expressed ρCe (T ) for these compounds as follows: ρCe (T ) = ρ0,Ce + ρLa (T ) − ρ0,La + ρf (T ), where ρ0,Ce , ρ0,La and ρCe , ρLa denote temperature-independent residual resistivity and total electrical resistivity of a compound with Ce and the corresponding isostructural analog with La. While analyzing the peculiarities of ρf (T ), the component ρ0 can be neglected and ρf (T ) ≈ ρCe (T ) − ρLa (T ) assumed. When deﬁning f -state contribution to the total thermoelectric power, the GorterNordheim relation [10,11] is usually used Sf (T ) =

(SCe ρCe − SLa ρLa ) , (ρCe − ρLa )

where SCe , SLa denote the total thermoelectric power of a compound with Ce and the corresponding isostructural analog with La. In our case we assumed that Sf (T ) ≈ SCe (T ) − SLa (T ). Such a ratio appears to be more convenient since the presence of the local structure gf (E) near the level EF is the domineering factor in forming the total thermoelectric power (SCe ) and frequently it is not domineering in the case of the total electrical resistivity (ρCe ). It is particularly characteristic of Ce compounds with transition 3d-elements [13].

3. Theoretical details Theoretically, the transport properties of the systems with the IV of Ce have been most logically studied by means of the Anderson model (AM) [5–7]. However, it has not been possible so far to derive analytical relationships allowing for a description of the behavior of the systems with transport properties using the Ce IV in a wide temperature range. This urged the development of various phenomenological approaches [8–13], based on a two-band model. According to [8–13], the main contribution to the transport properties was caused by scattering the electrons from a broad s(d)-band to a narrow f -band of Lorentzian shape. The scattering process can be described by the relaxation time in the form of τsf (E, T )−1 ∝ gf (E)Rph (T ). The function Rph (T ) takes into account the possible phonon-induced interband s-f transition. From the linearized Boltzmann transport equation, the following expressions for electrical resistivity component and thermoelectric power connected with the IV of Ce have been 1 1 1 L1 ρf (T ) = 2 , Sf (T ) = − , e L0 |e| L0 ∞ ∂f n dE, n = 0, 1, E τsf (E, T ) − Ln = ∂E −∞

267

M.D.Koterlyn, R.I.Yasnitskii, B.S.Morokhivskii

where f (E) is the Fermi-Dirac distribution function. The contribution of such s-f transitions to thermoelectric power in the approximation of an independent scattering on f -centers can be written as [13,17] Sf (T ) =

T εf 2 2 kB , π 2 3 |e| (π /3)T 2 + ε2f + Γ2f

(1)

where εf and Γf are the position of the gf (E) peak relative to the Fermi level EF and its width, respectively. Parameter kB is the Boltzmann constant. Equation (1) satisfactorily describes the temperature dependences of thermoelectric power of the majority of systems with IV of Ce even without taking into account the possible temperature dependences of the parameters εf and Γf . However, the parameters of the gf (E) peak determined from equation (1) do not quite agree with those determined based on the measurements of thermodynamic and spectroscopic characteristics [2,18,19]. The relationship between the parameters εf and Γf considerably deviates from that assumed in the AM [6] or in the local Fermi-liquid model [20] (by the thermopower data εf /Γf < 1 [8,9,13,17] when theoretical εf /Γf > 1). In the case of strong orbital degeneracy of f -states (Nf 1), which occurs in systems with intermediate Ce valence, it is appropriate to use the well-known relation connecting the parameters εf , Γf and TK (εf ≈ TK and Γf ≈ πTK /Nf [6]). Then, in place of equation (1), we obtain a more convenient expression, Sf (T ) =

2 2 kB T · TK , π 2 2 3 |e| (π /3)T + (1 + π 2 /Nf2 )TK2

(2)

with only one ﬁtting parameter TK . Recently we have shown [12] that a good agreement of the thermoelectric power curves calculated by equation (2) with the experimental data can be obtained only when the temperature dependence of the parameter TK is taken into account. This especially holds true for systems with the IV states of Ce, which are sensitive to temperature. There arises an important problem of realistic estimations of the temperature behavior of TK and their possible usage when describing electrical resistivity within the framework of the accepted model. With the aim of getting some idea of the behavior of the calculation ρf (T ), in order to describe the contribution of phonon-induced interband s-f transition to the resistance we use the simplest two-band spherical Mott–Wilson model [21] widely employed in nonmagnetic transition metals with an incomplete d shell. Taking into consideration only the N-process and temperature independent values of a matrix element for phonon induced s-f transition, we receive R0 · Rph (T ) , + (1 + π 2 /Nf2 )TK2 3 T θD −1 , Rph (T ) = ns (T ) J3 θD T ρf (T ) =

268

(π 2 /3)T 2

(3) (4)

Electronic transport properties of compounds . . .

where θD is the Debye temperature, R0 is the coeﬃcient taking into account a number of characteristic parameters of the model [21], ns (T ) is the eﬀective number of s electrons per atom depending on the temperature caused by the changes of f state occupation. The functions J3 (x) are the well-known transport integrals deﬁned by x y 3dy J3 (x) = . y −y 0 (e − 1)(1 − e ) Due to the special sensitivity of thermoelectric power to the parameters of the ﬁne structure density of states, a detailed concordance of the calculation with the experiment was carried out only for the Sf (T ) component. The values of Sf calculated by equation (2) were normalized by the coeﬃcient p = Sf max,exp /Sf max,calc , where Sf max,exp and Sf max,calc denote the maximal values of the experimental thermoelectric power and the calculated one. The parameter p takes into account the discrepancy between the experimental values of Sf (T ) and those calculated without allowing in (2) for the concentration of scattering f -centers and the presence of other scattering mechanisms in the compound under study [22]. The dependences TK (T ), obtained due to such a concordance, were used for the estimation of ρf (T ) and some other crystal physical characteristics.

4. Results and analysis According to spectroscopic measurements [23], transition of Ce from a state with strongly mixed valence (Ce3.2+ ) to almost magnetic one (Ce3+ ) is observed in CeNi in the temperature range T < 300 K. The similar decrease of the Ce valence (≈ 0.1 − 0.2) takes place in the case of CeNi2 and CeNi2 Si2 reaching the state of Ce3.1+ [23,24]. Temperature dependences of the f -states of Ce contribution to the total thermoelectric power (Sf ) for compounds CeNi, CeNi2 and CeNi2 Si2 are presented in ﬁgure 1. Apparently, typical features of the Sf (T ) dependence for the compounds in question appear to be the presence of asymmetric maximum (qualitatively Sf ∼ T at T < TSf max and Sf ∼ T −1 at T > TSf max ) and a certain deviation from linear behavior Sf ∼ T at low T with the occurrence of positive curvature. A good agreement of the calculated thermoelectric power (ﬁgure 1, solid curve) with the experiment is reached when the temperature dependence of the parameter TK is considered (ﬁgure 2). In the low temperature range (T < TSf max ), the parameter TK sharply increases until values TK ≈ (2 − 5)TSf max . Linearity of the dependence Sf (T ) at T < TSf max frequently observed in such systems [2,8,13] is achieved only at TK = const according to equation (2). Such a dependence is shown for CeNi2 Si2 (ﬁgure 1, dotted curve calculated at TK = 680 K). The appearance of the positive curvature on the dependence of Sf (T ) in the low temperature range and the corresponding increase of TK (ﬁgure 2) makes it possible to coordinate the parameters of the resonant structure gf (E) with the main thermodynamic properties of crystals.

269

M.D.Koterlyn, R.I.Yasnitskii, B.S.Morokhivskii

Figure 1. Temperature dependences of the contribution of Ce f -states to the total thermopower of CeNi (1), CeNi2 (2) and CeNi2 Si2 (3). Solid lines plot thermopower calculated from equation (2) in the suggested temperature dependence of parameter TK and TK = const (dotted curve).

Figure 2. Temperature dependences of the parameter TK of CeNi (1), CeNi2 (2) and CeNi2 Si2 (3), obtained based on the agreement of experimental thermoelectric power with that calculated by equation (2).

270

Electronic transport properties of compounds . . .

It is well known [6,25] that the majority of thermodynamic properties of the systems with the IV of Ce are satisfactorily described within the framework of a single impurity Anderson model with allowing for strong orbital degeneration µ2 nf (0) 3TK (0)

(5)

π 2 kB2 nf (0) , 3TK (0)

(6)

χ(0) = and γ(0) =

where µ2 = gJ2 J(J + 1)µ2B is the eﬀective magnetic moment of the cerium 4f 1 state, nf (0) and TK (0) is the electronic occupation of f -states of Ce and singleion Kondo temperature, respectively, at low temperatures. To assess the values of TK (0) we use the known data [23] for the occupation of f -states of Ce in CeNi (nf (0) = 0.88) determined at T = 80 K. To deduct the contributions of d-states of Ni to the values of coeﬃcients γ(0) and χ(0), it is possible to use the similar data for LaNi. According to the data [26,27], γ(0) = 65 mJ·mol−1 (CeNi), 5 mJ·mol−1 (LaNi); χ(0) = 2.2 · 10−3 emu·mol−1 (CeNi), 0.2 · 10−3 emu·mol−1 (LaNi). After substitution of the data presented in equations (5) and (6), we obtain TK (0) = 350 and 390 K, correspondingly. Results of the estimation of TK (0) are in a good agreement with those determined by means of the thermoelectric power at low temperatures (we obtain TK (0) = 360 K at T = 15 K). A similar assessment carried out for CeNi2 in [19] gives TK (0) = 1500 K, which is also in a fair agreement with our calculations (we obtain TK (0) = 1450 K by the thermoelectric power data at T = 15 K).

Figure 3. Temperature dependences of the contribution of Ce f -states to the total electrical resistivity of CeNi (1) and CeNi2 Si2 (2). Lines plot calculated dependences according to equation (3). 271

M.D.Koterlyn, R.I.Yasnitskii, B.S.Morokhivskii

The experimental and calculated (solid curves) dependences of the component ρf (T ) are shown in ﬁgure 3. The component for CeNi2 is not given, LaNi2 being an unsuitable analogue for singling out a phonon component of electrical resistivity. Calculation of normalized resistivity ρf (T )/R0 was carried out by equation (3) with the use of the found dependence TK (T ) and additionally taking into account the residual electrical resistivity ρf (0), taken from the experiment. The coeﬃcient R0 is chosen such that the numerical value of ρf max /R0 agrees with the experimental data. In the case of CeNi, the best agreement between the calculation and the experiment is reached when the function Rph (T ) in equation (3) has the form of equation (4) with θD = 110 K and dependence ns (T ) = ns (0) + 0.7 · 10−4 T − 0.5 · 10−2 T 1/2 , found with the spectroscopic data [23]. In case of CeNi2 Si2 , the best concordance with the experiment is achieved only assuming Rph (T ) = const. The necessity of taking into account the temperature dependence of the time relaxation testiﬁes to a considerable eﬀect of electron-phonon interaction in CeNi on ρf (T ) behavior. This fact agrees with an anomalously strong interaction of the electron system with lattice vibrations revealed previously [28]. In the case of CeNi2 Si2 , the behavior type of ρf (T )corresponds to the Mott scattering on s-f -transitions with allowing for the temperature narrowing of the peak density of states gf (E). Some discrepancy of the calculation with the experiment for CeNi2 Si2 in the low temperature range can be caused by partial display of coherent eﬀects.

5. Conclusions By the set of the data presented one can conclude that the transport properties of the compounds with the temperature unstable IV of Ce can be satisfactorily described in a wide temperature range within the framework of a simple model of a narrow peak of the density of states gf (E) of Lorentzian shape with allowing for its narrowing caused by stabilization of the Ce3+ states as the temperature increases. The values of TK obtained at a low temperature are completely realistic and in a good agreement with the assessments made by other methods. The diﬀerences in the character of temperature dependences of electrical resistivity for CeNi and CeNi2 Si2 are probably caused by diﬀerent roles of band states played at forming IV of Ce.

References 1. 2. 3. 4. 5. 6. 7.

272

Stewart G.R. // Rev. Mod. Phys., 1984, vol. 56, p. 755. Brandt N.B., Moshchalkov V.V. // Adv. Phys., 1984, vol. 33, p. 373. Cornut D., Coqblin B. // Phys. Rev. B, 1972, vol. 5, p. 4541. Bhattacharjee A.K., Coqblin B. // Phys. Rev. B, 1976, vol. 13, p. 3441. Fischer K.H. // Z. Phys. B. – Cond. Matt., 1989, vol. 76, p. 315. Bickers N.E., Cox D.L., Wilkins J.W. // Phys. Rev. B, 1987, vol. 36, p. 2036. Zlatic V., Horvatic B., Milat I., Coqblin B., Czycholl G., Grenzebach C. // Phys. Rev. B, 2003, vol. 68, p. 104432.

Electronic transport properties of compounds . . .

8. Gottwick U., Gloos K., Horn S., Steglich F., Grewe N. // J. Magn. Magn. Mater., 1985, vol. 47,48, p. 536. 9. Garde G.S., Ray J. // Phys. Rev. B, 1995, vol. 51, p. 2960. 10. Koterlyn M.D., Babych O.I., Koterlyn G.M. // J. Alloys Comp., 2003, vol. 348, p. 52. 11. Koterlyn M.D., Babych O.I., Yasnitskii R.I. // Fiz. Tverd. Tela (St. Petersburg), 2002, vol. 44, p. 792 (in Russian). 12. Koterlyn M.D., Yasnitskii R.I., Koterlyn G.M., Morokhivskii B.S. // J. Alloys Comp., 2003, vol. 348, p. 52. 13. Koterlyn M.D., Babych O.I., Lutsiv R.V., Nemoshkalenko V.V., Nikolajev L.I., Jushchenko A.V. Preprint, No. 11, IMF, Kijev, 1986. 14. Lutsiv R.V., Koterlyn M.D., Babych O.I. // Fiz. Tverd. Tela (Leningrad), 1984, vol. 26, p. 1781 (in Russian). 15. Levin E.M., Lutsiv R.V., Finkelshtein L.D., Samsonova N.D., Yasnitskii R.I. // Fiz. Tverd. Tela (Leningrad), 1981, vol. 23, p. 2401 (in Russian). 16. Koterlyn M.D., Lutsiv R.V., Yasnitskii R.I. // Ukr. Fiz. Jurn., 1984, vol. 29, p. 1587 (in Russian). 17. Koterlyn M.D., Lutsiv R.V. Physics and Chemistry of Rare-Earth Semiconductors. Novosibirsk, Nauka, 1990, p. 18. 18. Murani A.P., Raphel R., Bowden Z.A., Eccleston R.S. // Phys. Rev. B, 1996, vol. 53, p. 8188. 19. Murani A.P., Eccleston R.S. // Phys. Rev. B, 1996, vol. 53, p. 48. 20. Newns D.M., Newson A.C. // J. Phys. F: Metal Phys., 1980, vol. 10, p. 2429. 21. Colquitt L. // J. Appl. Phys., 1965, vol. 36, p. 2454. 22. Lutsiv R.V., Koterlyn M.D. // Fiz. Tverd. Tela (Leningrad), 1983, vol. 25, p. 2484 (in Russian). 23. Sovestnov A.E., Shaburov V.A., Markova J.A., Savitskii E.M., Chistjakov O.D., Shkatova T.M. // Fiz. Tverd. Tela (Leningrad), 1981, vol. 23, p. 2827 (in Russian). 24. Groshev M.N., Koterlyn M.D., Levin E.M., Lutsiv R.V., Miftahov N.M., Smirnov Yu.P., Sovestnov A.E., Tyunis A.V., Shaburov V.A., Yasnitskii R.I., Kuzmina S.M., Petrova V.I., Tyukavin V.A. // Fiz. Tverd. Tela (Leningrad), 1986, vol. 28, p. 2711 (in Russian). 25. Ramakrishnan T.V., Sur K. // Phys. Rev. B, 1982, vol. 26, p. 1798. 26. Gignoux D., Givord F., Lemaire R., Tasset F. // J. Less-Common. Met., 1983, vol. 94, p. 165. 27. Isikawa Y., Mori K., Fujii A., Sato K. // J. Phys. Soc. Jap., 1986, vol. 55, p. 3165. 28. Clementyev E.S., Braden M., Lasukov V.N., Alekseev P.A., Mignot J.-M., Sadikov I.P., Hiess A., Lapertot G. // Physica B: Cond. Matter., 1999, vol. 259–261, p. 42.

273

M.D.Koterlyn, R.I.Yasnitskii, B.S.Morokhivskii

Eлeктронні транcпортні влаcтивоcті cполук з тeмпeратурно-нecтабільною проміжною валeнтніcтю Ce М.Д.Kотeрлин 1,2 , Р.Й.Яcницький 1 , Б.C.Морохівcький 1 Львівcький національний унівeрcитeт імeні Івана Франка, вул. Драгоманова 50, 79-005, Львів, Україна 2 Акадeмія Бидгощcка, пл. Вeйcceнгоффа 11, 85-072 Бидгощ, Польща 1

Отримано 12 бeрeзня 2004 р. Для cполук CeNi, CeNi2 та CeNi2 Si2 прeдcтавлeні рeзультати вимірювання в інтeрвалі тeмпeратур 4–800 K cкладових тeрмо-e.р.c. (Sf ) та eлeктроопору (ρf ), викликаних тeмпeратурно-нecтабільною проміжною валeнтніcтю Ce. Показано, що залeжноcті Sf (T ) та ρf (T ) в широкому інтeрвалі тeмпeратур добрe опиcуютьcя на оcнові проcтої модeлі вузького піку гуcтини cтанів gf (E) лорeнцівcької форми біля рівня Фeрмі. Ширина піку залeжить від тeмпeратури і визначаєтьcя одно-іонною тeмпeратурою Kондо TK . Ключові слова: рідкіcнозeмeльні cполуки, валeнтні флуктуації, eлeктроопір, тeрмоeлeктрорушійна cила PACS: 72.20.Lp, 72.10. Fk, 72.15.Qm, 75.30.Mb

274

Electronic transport properties of compounds with temperature unstable intermediate valence of Ce M.D.Koterlyn ∗ 1,2 , R.I.Yasnitskii 1 , B.S.Morokhivskii 1 1

Ivan Franko National University of Lviv, Dragomanova Str. 50, 79005 Lviv, Ukraine

2

Academy of Bydgoszcz, Sq. Weyssenhoffa 11, 85-072 Bydgoszcz, Poland

Received March 12, 2004 Results of a thermoelectric power component (Sf ) and electrical resistivity (ρf ) measurements connected with the temperature unstable intermediate valence of Ce are presented for CeNi, CeNi2 and CeNi2 Si2 compounds in the temperature range 4–800 K. It is shown that dependences Sf (T ) and ρf (T ) are well described in a wide temperature range within the framework of a simple model of a narrow peak in the density of states gf (E) of Lorentzian shape near the Fermi level. The width of the peak depends on temperature and defines the characteristic single-ion Kondo temperature TK . Key words: rare earth compounds, valence fluctuation, electrical resistivity, thermoelectric power PACS: 72.20.Lp, 72.10.Fk, 75.30.Mb

1. Introduction Metallic systems containing rare-earth elements with unstable 4f -electronic states have been very attractive for the last decades. A speciﬁc feature of this class of compounds turns out to be the anomalously high values of certain physical characteristics, e.g., the coeﬃcient γ of the electronic-speciﬁc heat, magnetic susceptibility χ, thermoelectric power S, that can exceed the values typical of simple metals by 10 − 103 times [1,2]. In the band energy representation, a formation of the resonance peaks of the density of f -states, gf (E), near the Fermi level EF with a width of the order of the characteristic single-ion Kondo temperature TK (the so-called Abrikosov-Suhl resonance [2]) corresponds to this phenomenon. Despite the presence of a large number of experimental and theoretical works devoted to the many-body ∗

E-mail: [email protected]

c M.D.Koterlyn E-mail: [email protected] , R.I.Yasnitskii, B.S.Morokhivskii

265

M.D.Koterlyn, R.I.Yasnitskii, B.S.Morokhivskii

eﬀect studies when the conduction electrons interact with the 4f electrons in the compounds of this class, the nature of the resonant structure of the gf (E) remains the main issue to be discussed in future. Of special interest herein there are the intermetallic compounds showing the temperature unstable intermediate valence (IV) of Ce. These are most suitable for a model description in a study of the formation mechanism of the gf (E) structure. Transport properties of metallic compounds containing Ce with unstable f electrons turn out to be most sensitive to the peculiarities of the near Fermi state spectrum and can be used as a “ﬁne instrument” while studying the nature of the ground state. It is known that transport characteristics of such systems can be described in the relaxation time approximation with allowing for the exchange scattering of conduction electrons on local f -states [3–5]. However, with a detailed consideration of a number of important factors, such as the f -state orbital degeneracy, crystal ﬁeld-split f -states, the f -state hybridization with the band electrons, many-body eﬀects connected with f -electron correlation eﬀects, one cannot succeed in obtaining a general solution of the transport coeﬃcient behavior problem in a wide temperature range [6,7]. Moreover, one cannot succeed in coordinating the results of description of the transport coeﬃcients with the data of measurements of other physical properties. All this contributed to the development of a number of phenomenological approaches to the description of transport properties of such systems [8–10]. However, detailed comparisons of calculation values of transport properties within the limits of approximations [8–10] with experimental ones in a wide temperature range have not been carried out yet. This caused an insuﬃcient study of the possible usage of such experimental data for the determined resonance structure gf (E) parameters in a wide temperature range. The given paper shows temperature dependences of the contribution of Ce f states to the total thermoelectric power (Sf ) and to the electrical resistivity (ρf ) for compounds CeNi, CeNi2 and CeNi2 Si2 with diﬀerent temperature stability IV of Ce. Based on the phenomenological approach oﬀered by us earlier [10–12] there was carried out the analysis of Sf (T ), ρf (T ) dependences as well as of the transformation of the resonance structure gf (E) near the Fermi level at temperature changes within the largest limits (4–800 K).

2. Experimental data Preparation of polycrystalline samples and methods of the performed measurements were described in pervious papers [13,14]. Transport properties of the compounds CeNi, CeNi2 , CeNi2 Si2 and the corresponding analogs with La were partially analysed by us earlier [13–16]. The thermoelectric power of compounds with Ce is positive and reveals a typical maximum. The electrical resistivity manifests essential discrepancies from the Bloch-Gr¨ uneisen law characteristic of the systems with IV of Ce. For compounds with La, the thermoelectric power and electrical resistivity behavior is similar to that observed in non-magnetic transition metals. Assuming that the resistivity of the lanthanum-based counterpart can be taken 266

Electronic transport properties of compounds . . .

as a good approximation of the phonon contribution to the total measured resistivity of CeNi, CeNi2 and CeNi2 Si2 we expressed ρCe (T ) for these compounds as follows: ρCe (T ) = ρ0,Ce + ρLa (T ) − ρ0,La + ρf (T ), where ρ0,Ce , ρ0,La and ρCe , ρLa denote temperature-independent residual resistivity and total electrical resistivity of a compound with Ce and the corresponding isostructural analog with La. While analyzing the peculiarities of ρf (T ), the component ρ0 can be neglected and ρf (T ) ≈ ρCe (T ) − ρLa (T ) assumed. When deﬁning f -state contribution to the total thermoelectric power, the GorterNordheim relation [10,11] is usually used Sf (T ) =

(SCe ρCe − SLa ρLa ) , (ρCe − ρLa )

where SCe , SLa denote the total thermoelectric power of a compound with Ce and the corresponding isostructural analog with La. In our case we assumed that Sf (T ) ≈ SCe (T ) − SLa (T ). Such a ratio appears to be more convenient since the presence of the local structure gf (E) near the level EF is the domineering factor in forming the total thermoelectric power (SCe ) and frequently it is not domineering in the case of the total electrical resistivity (ρCe ). It is particularly characteristic of Ce compounds with transition 3d-elements [13].

3. Theoretical details Theoretically, the transport properties of the systems with the IV of Ce have been most logically studied by means of the Anderson model (AM) [5–7]. However, it has not been possible so far to derive analytical relationships allowing for a description of the behavior of the systems with transport properties using the Ce IV in a wide temperature range. This urged the development of various phenomenological approaches [8–13], based on a two-band model. According to [8–13], the main contribution to the transport properties was caused by scattering the electrons from a broad s(d)-band to a narrow f -band of Lorentzian shape. The scattering process can be described by the relaxation time in the form of τsf (E, T )−1 ∝ gf (E)Rph (T ). The function Rph (T ) takes into account the possible phonon-induced interband s-f transition. From the linearized Boltzmann transport equation, the following expressions for electrical resistivity component and thermoelectric power connected with the IV of Ce have been 1 1 1 L1 ρf (T ) = 2 , Sf (T ) = − , e L0 |e| L0 ∞ ∂f n dE, n = 0, 1, E τsf (E, T ) − Ln = ∂E −∞

267

M.D.Koterlyn, R.I.Yasnitskii, B.S.Morokhivskii

where f (E) is the Fermi-Dirac distribution function. The contribution of such s-f transitions to thermoelectric power in the approximation of an independent scattering on f -centers can be written as [13,17] Sf (T ) =

T εf 2 2 kB , π 2 3 |e| (π /3)T 2 + ε2f + Γ2f

(1)

where εf and Γf are the position of the gf (E) peak relative to the Fermi level EF and its width, respectively. Parameter kB is the Boltzmann constant. Equation (1) satisfactorily describes the temperature dependences of thermoelectric power of the majority of systems with IV of Ce even without taking into account the possible temperature dependences of the parameters εf and Γf . However, the parameters of the gf (E) peak determined from equation (1) do not quite agree with those determined based on the measurements of thermodynamic and spectroscopic characteristics [2,18,19]. The relationship between the parameters εf and Γf considerably deviates from that assumed in the AM [6] or in the local Fermi-liquid model [20] (by the thermopower data εf /Γf < 1 [8,9,13,17] when theoretical εf /Γf > 1). In the case of strong orbital degeneracy of f -states (Nf 1), which occurs in systems with intermediate Ce valence, it is appropriate to use the well-known relation connecting the parameters εf , Γf and TK (εf ≈ TK and Γf ≈ πTK /Nf [6]). Then, in place of equation (1), we obtain a more convenient expression, Sf (T ) =

2 2 kB T · TK , π 2 2 3 |e| (π /3)T + (1 + π 2 /Nf2 )TK2

(2)

with only one ﬁtting parameter TK . Recently we have shown [12] that a good agreement of the thermoelectric power curves calculated by equation (2) with the experimental data can be obtained only when the temperature dependence of the parameter TK is taken into account. This especially holds true for systems with the IV states of Ce, which are sensitive to temperature. There arises an important problem of realistic estimations of the temperature behavior of TK and their possible usage when describing electrical resistivity within the framework of the accepted model. With the aim of getting some idea of the behavior of the calculation ρf (T ), in order to describe the contribution of phonon-induced interband s-f transition to the resistance we use the simplest two-band spherical Mott–Wilson model [21] widely employed in nonmagnetic transition metals with an incomplete d shell. Taking into consideration only the N-process and temperature independent values of a matrix element for phonon induced s-f transition, we receive R0 · Rph (T ) , + (1 + π 2 /Nf2 )TK2 3 T θD −1 , Rph (T ) = ns (T ) J3 θD T ρf (T ) =

268

(π 2 /3)T 2

(3) (4)

Electronic transport properties of compounds . . .

where θD is the Debye temperature, R0 is the coeﬃcient taking into account a number of characteristic parameters of the model [21], ns (T ) is the eﬀective number of s electrons per atom depending on the temperature caused by the changes of f state occupation. The functions J3 (x) are the well-known transport integrals deﬁned by x y 3dy J3 (x) = . y −y 0 (e − 1)(1 − e ) Due to the special sensitivity of thermoelectric power to the parameters of the ﬁne structure density of states, a detailed concordance of the calculation with the experiment was carried out only for the Sf (T ) component. The values of Sf calculated by equation (2) were normalized by the coeﬃcient p = Sf max,exp /Sf max,calc , where Sf max,exp and Sf max,calc denote the maximal values of the experimental thermoelectric power and the calculated one. The parameter p takes into account the discrepancy between the experimental values of Sf (T ) and those calculated without allowing in (2) for the concentration of scattering f -centers and the presence of other scattering mechanisms in the compound under study [22]. The dependences TK (T ), obtained due to such a concordance, were used for the estimation of ρf (T ) and some other crystal physical characteristics.

4. Results and analysis According to spectroscopic measurements [23], transition of Ce from a state with strongly mixed valence (Ce3.2+ ) to almost magnetic one (Ce3+ ) is observed in CeNi in the temperature range T < 300 K. The similar decrease of the Ce valence (≈ 0.1 − 0.2) takes place in the case of CeNi2 and CeNi2 Si2 reaching the state of Ce3.1+ [23,24]. Temperature dependences of the f -states of Ce contribution to the total thermoelectric power (Sf ) for compounds CeNi, CeNi2 and CeNi2 Si2 are presented in ﬁgure 1. Apparently, typical features of the Sf (T ) dependence for the compounds in question appear to be the presence of asymmetric maximum (qualitatively Sf ∼ T at T < TSf max and Sf ∼ T −1 at T > TSf max ) and a certain deviation from linear behavior Sf ∼ T at low T with the occurrence of positive curvature. A good agreement of the calculated thermoelectric power (ﬁgure 1, solid curve) with the experiment is reached when the temperature dependence of the parameter TK is considered (ﬁgure 2). In the low temperature range (T < TSf max ), the parameter TK sharply increases until values TK ≈ (2 − 5)TSf max . Linearity of the dependence Sf (T ) at T < TSf max frequently observed in such systems [2,8,13] is achieved only at TK = const according to equation (2). Such a dependence is shown for CeNi2 Si2 (ﬁgure 1, dotted curve calculated at TK = 680 K). The appearance of the positive curvature on the dependence of Sf (T ) in the low temperature range and the corresponding increase of TK (ﬁgure 2) makes it possible to coordinate the parameters of the resonant structure gf (E) with the main thermodynamic properties of crystals.

269

M.D.Koterlyn, R.I.Yasnitskii, B.S.Morokhivskii

Figure 1. Temperature dependences of the contribution of Ce f -states to the total thermopower of CeNi (1), CeNi2 (2) and CeNi2 Si2 (3). Solid lines plot thermopower calculated from equation (2) in the suggested temperature dependence of parameter TK and TK = const (dotted curve).

Figure 2. Temperature dependences of the parameter TK of CeNi (1), CeNi2 (2) and CeNi2 Si2 (3), obtained based on the agreement of experimental thermoelectric power with that calculated by equation (2).

270

Electronic transport properties of compounds . . .

It is well known [6,25] that the majority of thermodynamic properties of the systems with the IV of Ce are satisfactorily described within the framework of a single impurity Anderson model with allowing for strong orbital degeneration µ2 nf (0) 3TK (0)

(5)

π 2 kB2 nf (0) , 3TK (0)

(6)

χ(0) = and γ(0) =

where µ2 = gJ2 J(J + 1)µ2B is the eﬀective magnetic moment of the cerium 4f 1 state, nf (0) and TK (0) is the electronic occupation of f -states of Ce and singleion Kondo temperature, respectively, at low temperatures. To assess the values of TK (0) we use the known data [23] for the occupation of f -states of Ce in CeNi (nf (0) = 0.88) determined at T = 80 K. To deduct the contributions of d-states of Ni to the values of coeﬃcients γ(0) and χ(0), it is possible to use the similar data for LaNi. According to the data [26,27], γ(0) = 65 mJ·mol−1 (CeNi), 5 mJ·mol−1 (LaNi); χ(0) = 2.2 · 10−3 emu·mol−1 (CeNi), 0.2 · 10−3 emu·mol−1 (LaNi). After substitution of the data presented in equations (5) and (6), we obtain TK (0) = 350 and 390 K, correspondingly. Results of the estimation of TK (0) are in a good agreement with those determined by means of the thermoelectric power at low temperatures (we obtain TK (0) = 360 K at T = 15 K). A similar assessment carried out for CeNi2 in [19] gives TK (0) = 1500 K, which is also in a fair agreement with our calculations (we obtain TK (0) = 1450 K by the thermoelectric power data at T = 15 K).

Figure 3. Temperature dependences of the contribution of Ce f -states to the total electrical resistivity of CeNi (1) and CeNi2 Si2 (2). Lines plot calculated dependences according to equation (3). 271

M.D.Koterlyn, R.I.Yasnitskii, B.S.Morokhivskii

The experimental and calculated (solid curves) dependences of the component ρf (T ) are shown in ﬁgure 3. The component for CeNi2 is not given, LaNi2 being an unsuitable analogue for singling out a phonon component of electrical resistivity. Calculation of normalized resistivity ρf (T )/R0 was carried out by equation (3) with the use of the found dependence TK (T ) and additionally taking into account the residual electrical resistivity ρf (0), taken from the experiment. The coeﬃcient R0 is chosen such that the numerical value of ρf max /R0 agrees with the experimental data. In the case of CeNi, the best agreement between the calculation and the experiment is reached when the function Rph (T ) in equation (3) has the form of equation (4) with θD = 110 K and dependence ns (T ) = ns (0) + 0.7 · 10−4 T − 0.5 · 10−2 T 1/2 , found with the spectroscopic data [23]. In case of CeNi2 Si2 , the best concordance with the experiment is achieved only assuming Rph (T ) = const. The necessity of taking into account the temperature dependence of the time relaxation testiﬁes to a considerable eﬀect of electron-phonon interaction in CeNi on ρf (T ) behavior. This fact agrees with an anomalously strong interaction of the electron system with lattice vibrations revealed previously [28]. In the case of CeNi2 Si2 , the behavior type of ρf (T )corresponds to the Mott scattering on s-f -transitions with allowing for the temperature narrowing of the peak density of states gf (E). Some discrepancy of the calculation with the experiment for CeNi2 Si2 in the low temperature range can be caused by partial display of coherent eﬀects.

5. Conclusions By the set of the data presented one can conclude that the transport properties of the compounds with the temperature unstable IV of Ce can be satisfactorily described in a wide temperature range within the framework of a simple model of a narrow peak of the density of states gf (E) of Lorentzian shape with allowing for its narrowing caused by stabilization of the Ce3+ states as the temperature increases. The values of TK obtained at a low temperature are completely realistic and in a good agreement with the assessments made by other methods. The diﬀerences in the character of temperature dependences of electrical resistivity for CeNi and CeNi2 Si2 are probably caused by diﬀerent roles of band states played at forming IV of Ce.

References 1. 2. 3. 4. 5. 6. 7.

272

Stewart G.R. // Rev. Mod. Phys., 1984, vol. 56, p. 755. Brandt N.B., Moshchalkov V.V. // Adv. Phys., 1984, vol. 33, p. 373. Cornut D., Coqblin B. // Phys. Rev. B, 1972, vol. 5, p. 4541. Bhattacharjee A.K., Coqblin B. // Phys. Rev. B, 1976, vol. 13, p. 3441. Fischer K.H. // Z. Phys. B. – Cond. Matt., 1989, vol. 76, p. 315. Bickers N.E., Cox D.L., Wilkins J.W. // Phys. Rev. B, 1987, vol. 36, p. 2036. Zlatic V., Horvatic B., Milat I., Coqblin B., Czycholl G., Grenzebach C. // Phys. Rev. B, 2003, vol. 68, p. 104432.

Electronic transport properties of compounds . . .

8. Gottwick U., Gloos K., Horn S., Steglich F., Grewe N. // J. Magn. Magn. Mater., 1985, vol. 47,48, p. 536. 9. Garde G.S., Ray J. // Phys. Rev. B, 1995, vol. 51, p. 2960. 10. Koterlyn M.D., Babych O.I., Koterlyn G.M. // J. Alloys Comp., 2003, vol. 348, p. 52. 11. Koterlyn M.D., Babych O.I., Yasnitskii R.I. // Fiz. Tverd. Tela (St. Petersburg), 2002, vol. 44, p. 792 (in Russian). 12. Koterlyn M.D., Yasnitskii R.I., Koterlyn G.M., Morokhivskii B.S. // J. Alloys Comp., 2003, vol. 348, p. 52. 13. Koterlyn M.D., Babych O.I., Lutsiv R.V., Nemoshkalenko V.V., Nikolajev L.I., Jushchenko A.V. Preprint, No. 11, IMF, Kijev, 1986. 14. Lutsiv R.V., Koterlyn M.D., Babych O.I. // Fiz. Tverd. Tela (Leningrad), 1984, vol. 26, p. 1781 (in Russian). 15. Levin E.M., Lutsiv R.V., Finkelshtein L.D., Samsonova N.D., Yasnitskii R.I. // Fiz. Tverd. Tela (Leningrad), 1981, vol. 23, p. 2401 (in Russian). 16. Koterlyn M.D., Lutsiv R.V., Yasnitskii R.I. // Ukr. Fiz. Jurn., 1984, vol. 29, p. 1587 (in Russian). 17. Koterlyn M.D., Lutsiv R.V. Physics and Chemistry of Rare-Earth Semiconductors. Novosibirsk, Nauka, 1990, p. 18. 18. Murani A.P., Raphel R., Bowden Z.A., Eccleston R.S. // Phys. Rev. B, 1996, vol. 53, p. 8188. 19. Murani A.P., Eccleston R.S. // Phys. Rev. B, 1996, vol. 53, p. 48. 20. Newns D.M., Newson A.C. // J. Phys. F: Metal Phys., 1980, vol. 10, p. 2429. 21. Colquitt L. // J. Appl. Phys., 1965, vol. 36, p. 2454. 22. Lutsiv R.V., Koterlyn M.D. // Fiz. Tverd. Tela (Leningrad), 1983, vol. 25, p. 2484 (in Russian). 23. Sovestnov A.E., Shaburov V.A., Markova J.A., Savitskii E.M., Chistjakov O.D., Shkatova T.M. // Fiz. Tverd. Tela (Leningrad), 1981, vol. 23, p. 2827 (in Russian). 24. Groshev M.N., Koterlyn M.D., Levin E.M., Lutsiv R.V., Miftahov N.M., Smirnov Yu.P., Sovestnov A.E., Tyunis A.V., Shaburov V.A., Yasnitskii R.I., Kuzmina S.M., Petrova V.I., Tyukavin V.A. // Fiz. Tverd. Tela (Leningrad), 1986, vol. 28, p. 2711 (in Russian). 25. Ramakrishnan T.V., Sur K. // Phys. Rev. B, 1982, vol. 26, p. 1798. 26. Gignoux D., Givord F., Lemaire R., Tasset F. // J. Less-Common. Met., 1983, vol. 94, p. 165. 27. Isikawa Y., Mori K., Fujii A., Sato K. // J. Phys. Soc. Jap., 1986, vol. 55, p. 3165. 28. Clementyev E.S., Braden M., Lasukov V.N., Alekseev P.A., Mignot J.-M., Sadikov I.P., Hiess A., Lapertot G. // Physica B: Cond. Matter., 1999, vol. 259–261, p. 42.

273

M.D.Koterlyn, R.I.Yasnitskii, B.S.Morokhivskii

Eлeктронні транcпортні влаcтивоcті cполук з тeмпeратурно-нecтабільною проміжною валeнтніcтю Ce М.Д.Kотeрлин 1,2 , Р.Й.Яcницький 1 , Б.C.Морохівcький 1 Львівcький національний унівeрcитeт імeні Івана Франка, вул. Драгоманова 50, 79-005, Львів, Україна 2 Акадeмія Бидгощcка, пл. Вeйcceнгоффа 11, 85-072 Бидгощ, Польща 1

Отримано 12 бeрeзня 2004 р. Для cполук CeNi, CeNi2 та CeNi2 Si2 прeдcтавлeні рeзультати вимірювання в інтeрвалі тeмпeратур 4–800 K cкладових тeрмо-e.р.c. (Sf ) та eлeктроопору (ρf ), викликаних тeмпeратурно-нecтабільною проміжною валeнтніcтю Ce. Показано, що залeжноcті Sf (T ) та ρf (T ) в широкому інтeрвалі тeмпeратур добрe опиcуютьcя на оcнові проcтої модeлі вузького піку гуcтини cтанів gf (E) лорeнцівcької форми біля рівня Фeрмі. Ширина піку залeжить від тeмпeратури і визначаєтьcя одно-іонною тeмпeратурою Kондо TK . Ключові слова: рідкіcнозeмeльні cполуки, валeнтні флуктуації, eлeктроопір, тeрмоeлeктрорушійна cила PACS: 72.20.Lp, 72.10. Fk, 72.15.Qm, 75.30.Mb

274